Anharmonic motions <i>versus</i> dynamic disorder at the Mg ion from the charge densities in pyrope (Mg~3~Al~2~Si~3~O~12~) crystals at 30K: six of one, half a dozen of the other
Destro, Riccardo; Ruffo, Riccardo; Roversi, Pietro; Soave, Raffaella; Loconte, Laura; Lo Presti, Leonardo; Acta Crystallographica Section B 73 (2017) 722–736; doi:10.1107/S2052520617006102

data_2108142
_publ_section_title
;
 Anharmonic motions <i>versus</i> dynamic disorder at the Mg ion from the
 charge densities in pyrope (Mg~3~Al~2~Si~3~O~12~) crystals at 30K: six of
 one, half a dozen of the other
;
_journal_coeditor_code           PI5032
_journal_issue                   4
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              722
_journal_page_last               736
_journal_paper_doi               10.1107/S2052520617006102
_journal_volume                  73
_journal_year                    2017
_chemical_formula_moiety         '2(AL) 3(MG) 3(SIO4)'
_chemical_formula_sum            'Al2 Mg3 O12 Si3'
_chemical_formula_weight         403.16
_chemical_name_common            pyrope
_space_group_crystal_system      cubic
_space_group_IT_number           230
_space_group_name_Hall           '-I 4bd 2c 3'
_space_group_name_H-M_alt        'I a -3 d'
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method
'Created with CONVERT.DLL (www.crystalimpact.com)'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.4405(3)
_cell_length_b                   11.4405(3)
_cell_length_c                   11.4405(3)
_cell_measurement_reflns_used    406
_cell_measurement_temperature    30.0(3)
_cell_measurement_theta_max      53.52
_cell_measurement_theta_min      11.01
_cell_volume                     1497.39(7)
_computing_structure_refinement
;
VALRAY2000 (Stewart, Spackman & Flensburg, 2000)'
;
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      30.0(3)
_diffrn_measured_fraction_theta_full 1.0
_diffrn_measurement_device_type  'Syntex P1-'
_diffrn_measurement_method       '2\q/\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0134
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            7486
_diffrn_reflns_theta_full        54.5
_diffrn_reflns_theta_max         54.5
_diffrn_reflns_theta_min         1.000
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 97
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    1.218
_exptl_absorpt_correction_T_max  0.6868
_exptl_absorpt_correction_T_min  0.6680
_exptl_absorpt_correction_type   sphere
_exptl_absorpt_process_details   'TBAR, home written program'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.576
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       sphere
_exptl_crystal_F_000             1600
_exptl_crystal_size_max          0.45
_exptl_crystal_size_mid          0.45
_exptl_crystal_size_min          0.45
_exptl_crystal_size_rad          0.45
_refine_diff_density_max         0.12
_refine_diff_density_min         -0.16
_refine_ls_extinction_coef       0.248
_refine_ls_extinction_method     'type 1'
_refine_ls_goodness_of_fit_ref   0.7596
_refine_ls_matrix_type           full
_refine_ls_number_parameters     93
_refine_ls_number_reflns         785
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.7596
_refine_ls_R_factor_all          0.0084
_refine_ls_R_factor_gt           0.0084
_refine_ls_shift/su_max          0.0013
_refine_ls_shift/su_mean         0.0001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0081
_refine_ls_wR_factor_ref         0.0081
_reflns_number_gt                785
_reflns_number_total             788
_reflns_threshold_expression     >0
_cod_data_source_file            pi5032sup1.cif
_cod_data_source_block           I
_cod_original_cell_volume        1497.39(12)
_cod_database_code               2108142